Article Materials Science
January 2011 Vol.56 No.1: 96–101 doi: 10.1007/s11434-010-4115-2
Application of upconversion luminescence in dye-sensitized solar cells XIE GuiXiang, LIN JianMing, WU JiHuai*, LAN Zhang, LI QingHua, XIAO YaoMing, YUE GenTian, YUE HaiFeng & HUANG MiaoLiang Engineering Research Center of Environment-Friendly Functional Materials, Ministry of Education, China; The Key Laboratory for Functional Materials of Fujian Higher Education, China; Institute of Material Physical Chemistry, Huaqiao University, Quanzhou 362021, China Received January 18, 2010; accepted July 22, 2010
An upconversion luminescence powder TiO2:(Er3+, Yb3+) is prepared by a hydrothermal method and used to fabricate dye-sensitized solar cell (DSSC). The TiO2:(Er3+, Yb3+) powder undergoes upconversion luminescence, converting infrared light which the dye can not absorb into visible light with wavelengths of 510–700 nm which the dye can absorb, increasing the photocurrent of the DSSC. TiO2:(Er3+, Yb3+) also acts as a p-type dopant, heightening the Fermi level of the oxide film, which increases the photovoltage of the DSSC. The best performance of the DSSC is found when the ratio of TiO2/luminescence powder is 1/3 in the luminescence layer. Under simulated solar irradiation of 100 mW cm–2 (AM 1.5), the DSSC containing TiO2:(Er3+, Yb3+) doping achieves a light-to-electricity energy conversion efficiency of 7.28% compared with 6.41% for the undoped DSSC. dye-sensitized solar cell, upconversion luminescence, p-type doping Citation:
Xie G X, Lin J M, Wu J H, et al. Application of upconversion luminescence in dye-sensitized solar cells. Chinese Sci Bull, 2011, 56: 96−101, doi: 10.1007/s11434-010-4115-2
In 1991, Gratzel’s group  reported a dye-sensitized solar cell with simple preparation procedure, low-cost, high efficiency and good stability, this new kinds of solar cell bring a revolutionary innovation for photoelectrichemical solar cell, and blaze a development direction for new generation’s solar cells. The conversion efficiency of DSSC can reach up to 11% . In DSSC, dyes N3 and N-719 often are used as photosensitized agents, and photoanodes together with TiO2 [1–5], therefore the solar light can be absorbed and transferred into electrical energy. The dye molecules can be regarded as an “electron pump”, the driving energy of the pump comes from the solar light. The mainly absorption wavelength ranges for dyes N3 and N-719 are 290–700 nm [3–5]. About 43% of the radiant energy from the sun in the infrared region is not absorbed, which limits the sun energy conversion efficiency of DSSC. It is significant for transferring infrared light to visible light which the dyes can absorb and enhancing the light-to-
electricity conversion efficiency of DSSC. Rare-earth-doped compounds have aroused extensive research as conversion luminescent mediums with potential applications in phosphors, display monitors, X-ray imaging, scintillators and solid-state lasers [6–10] because of their unique properties arising from their 4f electrons. However, using rare-earth-doped compounds for upconversion luminescence in DSSC has not been attempted so far. In this paper, a luminescent TiO2:(Er3+, Yb3+) powder is prepared by a hydrothermal method and used to fabricate a DSSC. TiO2:(Er3+, Yb3+) behaves as an upconversion luminescence medium, transferring infrared light to visible light which the dye can absorb, enhancing the light-to-electricity conversion efficiency of the DSSC.
*Corresponding author (email: [email protected]
TiO2 nanoparticles (P25), butyl titanate, isopropanol, iodine,
© The Author(s) 2011. This article is published with open access at Springerlink.com
1 Materials and methods 1.1
Materials and apparatus
Xie G X, et al.
Chinese Sci Bull
lithium iodide, polyglycol M-20,000, 4-tert-butyl-pyridine (TBP), Triton X-100, ytterbium oxide (Yb2O3) and erbium oxide (Er2O3) were purchased from the Shanghai Chemical Agent Ltd., China (Analytical purity grade). The dye N-719 [RuL2 (NCS)2, L=4,4’-dicarboxylate-2,2’-bipyridine)] was purchased from Solaronix SA, Switzerland. Other reagents were from Shanghai Chemical Agent Ltd., China. Conducting glass with a fluorine-doped tin oxide layer (FTO glass) with a sheet resistance of 15 Ω cm2 was purchased from Hartford Glass Co. This was used as a substrate for precipitation of a TiO2 porous film and was cut into rectangles with a size of 2 cm × 1.5 cm. The mainly apparatus include in a stabilized power supply Xe/Hg arc lamp (CHF-XM500W, Changtuo Scientific Ltd, Beijing, China) an electrochemical workstation (CHI660C, Shanghai Chenhua Device Company, China), an X-ray diffractometer (Bruker D8 Advance, Germany), an UV-Vis 2550 spectrophotometer and a Spectrofluorometer (FSP920, Edinburgh Instruments). 1.2
Preparation of TiO2 nanocrystal colloid
Using tetrabutyl titanate as precursor, a TiO2 nanocrystal colloid was prepared by the following procedure [11–14]. Tetrabutyl titanate (10 mL) was rapidly added to distilled water (150 mL), immediately forming a white precipitate. The system was stirred for 30 min. The precipitate was filtered using a glass frit and washed three times with 100 mL of distilled water. The precipitate was added to an aqueous solution of nitric acid (0.1 mol L–1, 100 mL) and stirred vigorously at 80°C until the slurry became a translucent bluewhite liquid. Thereinto 70 mL resultant colloidal suspension was autoclaved at 200°C for 12 h to form a white, milky slurry. The autoclaved 70 mL slurry was added to original blue-white liquid, adding 0.2 g TiO2 powder (P25), stirring 30 min, and then the second time hydrothermal treatment was conducted. The resultant slurry was concentrated to 1/5 of its original volume, then PEG-20,000 (20 wt%–30 wt% slurry) and a few drops of emulsification reagent Triton X-100  were added to form a stable TiO2 nanocrystal colloid. 1.3
Preparation of upconversion luminescence colloid
A TiO2:(Er3+, Yb3+) powder was prepared by the following process. Some of Er2O3, Yb2O3 and LiOH (as melt reagent)  were first dissolved in nitric acid (10 wt%) to form a nitrate solution. Meanwhile, 10 mL of tetrabutyl titanate was added to 150 mL of vigorously stirred distilled water, immediately forming a white precipitate. The system was stirred for 30 min. The precipitate was filtered using a glass frit and washed three times. The resulted precipitate was added into the nitrate solution, the pH of the mixed solution was adjusted to 1 by adding acetic acid (10 mL) and distilled water. The system was stirred at 80°C until a translucent blue-white colloid formed. The resultant colloid was autoclaved (filled less than 80%) at 200°C for 12 h to form
January (2011) Vol.56 No.1
a white precipitate containing Er3+ and Yb3+. After the precipitate was vacuum dried at 100°C, ground, calcined at 800°C for 2.5 h and cooled to room temperature, an upconversion luminescence powder was obtained. The upconversion luminescence powder was added to the TiO2 colloid in different ratios and concentrated at 80°C. then PEG-20000 (20 wt%–30 wt% slurry) and a few drops of Triton X-100 were added to form a stable upconversion luminescence colloid. 1.4
Preparation of upconversion luminescence electrode
Plastic adhesive tape was fixed on the four sides of the cleaned FTO conducting glass plate to restrict  the thickness of 10 μm and the area of 1 cm ×1 cm for the oxide film. The TiO2 colloid was dropped on the FTO glass plate using a scalpel. The resulting films were sintered at 450°C in air for 30 min to solidify the TiO2 film and delete organic impurity on the film, after cooling down to 80°C, a normal TiO2 film was obtained. By using the same method, an upconversion luminescence layer with thickness of 4 μm was covered on the TiO2 film. The resultant film was immersed in a 3×10–4 mol L–1 solution of N-719 in absolute ethanol for 24 h to adequately absorb the dye. The dye-sensitized oxide film was washed with anhydrous ethanol and dried in moisture-free air in dark to give a dye-sensitized upconversion luminescence electrode. 1.5
The phase and crystal structure of TiO2:(Er3+, Yb3+) upconversion luminescence powders were checked with an X-ray diffractometer (Bruker D8 Advance, Germany) using Cu Kα radiation (λ = 1.5405 Å) under 40 kV, 40 mA, and scan rate: 3°/min, scan range: 10°–80°. UV-Vis absorption spectrum of dye was measured using a UV-Vis 2500 spectrophotometer (Shimadzu Corporation, Japan). The photoluminescence (emission and excitation) spectra of the upconversion luminescence powders were measured on a spectrofluorometer (FSP920, Edinburgh Instruments). Photoelectric properties of the DSSCs were measured with an electrochemical workstation (CHI660C, Shanghai Chenhua Device Company, China) and a stabilized power supply Xe/Hg arc lamp (CHF-XM-500W, Changtuo Scientific Ltd, Beijin, China). 1.6
DSSC assemblage and photoelectric measurements
A DSSC was assembled by injecting an electrolyte into the aperture between the TiO2 film electrode (anode electrode) and a Pt-coated counter electrode . The electrolyte was consisted of 0.60 mol L–1 tetrabutyl ammonium iodide, 0.10 mol L–1 I2, and 0.50 mol L–1 4-tert-butyl-pyridine in acetonitrile. Using the stabilized power supply Xe/Hg arc lamp as a solar light simulator, controlling the incident light intensity
Xie G X, et al.
Chinese Sci Bull
(Pin) of 100 mW cm–2, the short circuit density (JSC, mA cm–2) and open circuit voltage (VOC, V) were measured using the electrochemical workstation (CHI660C, Shanghai Chenhua Device Company, China). The fill factor (FF) and the light-to-electricity conversion efficiency (η) of the DSSC were calculated according to the following equations :
η (%) =
Vmax × J max V × J × FF × 100% = OC SC × 100%, (1) Pin Pin FF =
Vmax × J max , VOC × J SC
where Jmax (mA cm–2) and Vmax (V) are the current density and voltage at the point of maximum power output on the J-V curves, respectively.
Results and discussion XRD patterns
The XRD patterns of the TiO2 and TiO2:(Er3+, Yb3+) powders are shown in Figure 1. Figure 1(a) shows that nearly all of the peaks correspond to the anatase phase (PDF No. 211272). Some of the rutile phase present in P25 is also observed. The anatase XRD peaks in Figure 1(a) are intense and well resolved, suggesting that the resultant TiO2 nanocrystals are highly crystalline. Nearly all of the anatase TiO2 changes to the rutile phase after calcination at 800°C for 2.5 (Figure 1(b)), because the signals after calcination are consistent with PDF card No. 65-0192. Figure 1(c) shows peaks resulting from the rutile phase of TiO2 in the TiO2:(Er3+, Yb3+) powder as well as some pyrochlore phases from Er2Ti2O7 and Yb2Ti2O7 (marked with p). The average diameters (D) of the particles can be calcu-
Figure 1 XRD patterns. (a) TiO2 nanocrystals after calcination at 450°C for 2.5 h; (b) TiO2 nanocrystals after calcination at 800°C for 2.5 h and (c) TiO2:(Er3+, Yb3+) powder.
January (2011) Vol.56 No.1
lated by the Scherrer formula : Dhkl =
kλ , β cos θ
where Dhkl is the particle size in the normal direction for (h k l) crystal face. Here, the constant K (depends on the particle shape, face index, β and Dhkl) adopts 0.9 . λ (0.1540 nm) is the wavelength of the Cu-Kα radiation, θ is the diffraction angle and β is the full width at half-maximum (FWHM in radians). According to Figure 1 and eq. (3), the apparent size D of the TiO2 nanocrystals in Figure 1(a) and the upconversion luminescence powders in Figure 1(c) are 19 nm and 68 nm, respectively. Compared with the diffraction peaks in curves (a) and (b), the intensity of diffraction peaks in curve (c) increase, indicating that the conversion luminescence powder has a higher crystallization and larger size, which the larger particles as light scattering points extend the light diffuse path, and enhance the incident photons capture efficiency . Meanwhile, it is known that the refractive index of the anatase phase is lower than that of the rutile phase (anatase: 2.5; rutile: 2.7). Thus TiO2:(Er3+, Yb3+) layer show a higher refractive index than undoped TiO2, which should help to increase light-to-electricity conversion efficiency of the DSSC. 2.2 Excitation and emission spectra of TiO2:(Er3+, Yb3+) Figure 2(a) shows the excitation spectra of the TiO2:(Er3+, Yb3+) powder. A strong, broad peak at 978 nm is observed. The band centered at 978 nm can be identified as the transition of Yb3+ from 2F7/2 to 2F5/2, indicating that the upconversion luminescence powder can effectively absorb the infrared light. The luminescence spectra of the TiO2:(Er3+, Yb3+) powder exhibits peaks in the green region from 510–570 nm and in the red region from 610–700 nm as shown in Figure 2(b). Upconversion fluorescence excitation can be readily observed with a 978 nm laser. The peaks centered at 521, 544 and 650 nm correspond to the Er3+: 2H11/2 → 4I15/2, 4S3/2 → 4 I15/2, and 4F9/2 → 4I15/2 [19–22] transitions, respectively. These upconversion luminescences, especially in 544 nm, are accorded with the absorption wavelength of the N-719. When doping the TiO2:(Er3+, Yb3+) powder in the photoanode of DSSC, it will effectively enhance the light-to-electricity efficiency of DSSC. Figure 3 shows the energy level diagram for Er3+ and Yb3+ codoped systems and upconversion luminescence process. The upconversion luminescence mechanism is shown as [20,22]: Yb3+ ions have a much larger absorption cross-section relative to that of Er3+ ions around 978 nm, so Yb3+ ions are excited preferentially. An Er3+ ion can then be excited from the 4I15/2 ground state to the 4I11/2 excited state by energy transfer from an excited Yb3+ ion. The Er3+ ion is
Xie G X, et al.
Chinese Sci Bull
January (2011) Vol.56 No.1
Figure 3 Energy levels of Er3+ and Yb3+ and upconversion transition pathways under 978-nm infrared excitation.
Figure 2 Excitation (a) and luminescence (b) spectra of TiO2:(Er3+, Yb3+) powders excited with a laser at 978 nm.
subsequently excited to the 4F7/2 state by absorbing energy from another Yb3+ ion. The Er3+ ion then decays nonradiatively to the 2H11/2, 4S3/2 and 4F9/2 levels. In addition, Er3+ ions in the 4I11/2 excited state can decay nonradiatively to the 4 I13/2 level and be excited to the 4F9/2 level by absorbing a second photon, resulting in green light emission (521 nm and 544 nm; 2H11/2 → 4I15/2 and 4S3/2 → 4I15/2, respectively). Alternatively, the Er3+ can further relax and populate the 4 F9/2 level leading to the red emission at 650 nm from the transition 4F9/2 → 4I15/2. 2.3
UV-Vis absorption spectrum
The UV-Vis absorption spectrum of the dye-sensitized TiO2 electrode is shown in Figure 4. A strong, broad absorption band occurs from 290 to 700 nm with a maximum at about 385 nm and a shoulder at 528 nm. It should be noted that the dye-sensitized TiO2 electrode cannot absorb light with wavelengths higher than 700 nm. According to the discussion on excitation and luminescence spectra, addition of TiO2:
UV-Vis absorption spectrum of a dye-sensitized TiO2 electrode.
(Er3+, Yb3+) powder into the TiO2 electrode should allow the infrared light with wavelength about 978 nm which the dye can not absorb transfers to the green light and the red light which the dye has a high absorption. Therefore, the more solar irradiation is absorbed by DSSC and the light-to-electricity conversion efficiency of the DSSC is increased. 2.4 Influence of upconversion luminescence on the photoelectric properties of DSSC To investigate the effect of infrared irradiation on DSSCs,
Xie G X, et al.
Chinese Sci Bull
we used a filter stop to remove the light of wavelength less than 720 nm. Figure 5 shows the photovoltaic characterization of the DSSCs with and without the upconversion luminescence powder under infrared irradiation of 60 mW cm−2. The DSSC lacking the upconversion luminescence powder possessed the photovoltaic parameters: JSC = 0.105 mA cm−2, VOC = 401 mV, FF = 0.560 and η = 0.04%. The DSSC containing the upconversion luminescence powder displays enhanced photovoltaic parameters: JSC = 0.248 mA cm−2, VOC = 561 mV, FF = 0.631 and η = 0.146%. The enhancement indicates that the upconversion luminescence layer can transfer infrared light to visible light which the N-719 dye can absorb effectively, increasing the harvested sunlight and improving the efficiency of the DSSC. The photocurrent-voltage curves of the DSSCs with and without an upconversion luminescence powder under simulated solar light irradiation of 100 mW cm–2 (AM 1.5) are shown in Figure 6. Table 1 shows the influence of the amount of the luminescence powder on the photoelectric properties of the DSSCs. As the amount of the luminescence powder in the DSSC increases, JSC increases and then decreases, and VOC increases. The maximum efficiency of the DSSC is achieved when the mass ratio of TiO2/luminescence powder is 1/3 in the luminescence layer. The increase in JSC with the amount of the luminescence powder at low concentrations is because the luminescence powder absorbs infrared light (978 nm) which it transfers to visible light (510–700 nm), resulting in an increase in incident light harvest, photoinduced electrons in unit area, and JSC in the DSSC. On the other hand, larger particle sizes in the upconversion luminescence layer extend the light transmission distance, improving the incident light harvest , and increasing the photocurrent. However, when Er3+ and Yb3+ are doped in TiO2, some crystal defects are present. The defects can capture photoinduced electrons and holes, leading to a decrease in photocurrent, especially in higher Er3+ and Yb3+ concentration. This explains why JSC increases and then decreases as the amount of TiO2:(Er3+, Yb3+) in the DSSC increases.
January (2011) Vol.56 No.1
Figure 6 Photocurrent-voltage curves of DSSCs with and without an upconversion luminescence layer. Table 1 Effects of an upconversion luminescence layer on the photoelectric properties of DSSCs JSC (mA cm–2)
1:0 1:1 1:2 1:3 1:4 1:5
15.40 15.57 15.92 15.45 13.35 10.91
0.717 0.718 0.724 0.748 0.799 0.817
0.580 0.598 0.588 0.629 0.611 0.633
6.41 6.68 6.81 7.28 6.52 5.64
According to Gratzel, VOC corresponds to the potential difference between the Fermi level of the electrons in the oxide film and the redox potential of the electrolyte [1,2]. When Er3+ and Yb3+ ions substitute Ti4+ ion lattice sites in TiO2, similar to Si semiconductors, i.e., p-type doping, the energy level of the oxide film is elevated, resulting in an increase of VOC. In our experiments, the electrolyte is the same so it is unsurprising that VOC increases as the amount of Er3+ and Yb3+ ions increase. When the mass ratio of TiO2/TiO2:(Er3+, Yb3+) is 1/5 in the luminescence layer, VOC reaches 0.817 V. This value is higher than that of other DSSCs with the same structure, showing significance of p-type doping for enhancing the photovoltage of DSSCs. Comprising JSC, VOC, FF and η, when the mass ratio of TiO2/TiO2:(Er3+, Yb3+) is 1/3 in the upconversion luminescence layer, the light-to-electricity conversion efficiency of the DSSC reaches 7.28%, which is an improvement of 13.6% compared with the DSSC not doped with rare-earth ions.
Figure 5 Photocurrent-voltage curves of the DSSCs with and without an upconversion luminescence layer under infrared irradiation.
TiO2/luminescence powder (mass ratio)
In summary, a TiO2:(Er3+, Yb3+) powder was synthesized using a hydrothermal method. The powder was used to fabricate an oxide film in the DSSCs. The rare-earth oxide undergoes upconversion luminescence, transferring infrared light (DSSC can not absorb) into visible light with wave-
Xie G X, et al.
Chinese Sci Bull
lengths of 510–700 nm (DSSC can absorb), enhancing the photocurrent of the DSSC. As a p-type dopant, the rareearth oxide increases the Fermi level of the oxide film and the photovoltage of DSSC. The highest efficiency of the DSSC is reached when the mass ratio of TiO2/TiO2:(Er3+, Yb3+) is 1/3 in the upconversion luminescence layer. Under a simulated solar light irradiation of 100 mW cm–2 (AM 1.5), the DSSC containing TiO2/TiO2:(Er3+, Yb3+) doping achieved a short-circuit current density of 15.45 mA cm–2, an open-circuit voltage of 0.748 V and a light-to-electricity conversion efficiency of 7.28%, which is enhanced by 13.6% compared with the DSSC lacking the luminescent layer. The present findings demonstrate the feasibility of rare-earth doping in DSSCs for providing an effective way to improve their sunlight conversion efficiency.
January (2011) Vol.56 No.1
14 This work was supported by the National High Technology Research and Development Program of China (2009AA03Z217) and the National Natural Science Foundation of China (90922028, 50842027).
1 2 3
O’Regan B, Gratzel M. A low-cost high-efficiency solar cell based on dye-sensitized colloidal TiO2 films. Nature, 1991, 353: 737–740 Gratzel M. Solar energy conversion by dye-sensitized photovoltaic cells. Inorg Chem, 2005, 44: 6841–6851 Gratzel M. Engineering of a novel ruthenium sensitizer and its application in dye-sensitized solar cells for conversion of sunlight into electricity. Inorg Chem, 2005, 44: 178–180 Lee S A, Abrams N M, Hoertz P G, et al. Compling of titania inverse opals to nanocrystalline titania layers in dye-sensitized solar cells. J Phys Chem B, 2008, 112: 14415–14421 Nazeeruddin M K, Kay A, Rodicio I, et al. Conversion of light to electricity by cis-bis (2, 2′-bipyridyl-4, 4′-dicarboxylate) ruthenium (II) charge-transfer sensitizers (X = Cl-, Br-, I-, CN-, and SCN-) on nanocrystalline TiO2 electrodes. J Am Chem Soc, 1993, 115: 6382– 6390 Wang W N, Widiyastuti W, Ogi T, et al. Correlations between crystallite/particle size and photoluminescence properties of submicrometer phosphors. Chem Mater, 2007, 19: 1723–1730 Yi G S, Lu H C, Zhao S Y, et al. Synthesis, characterization, and biological application of size-controlled nanocrystalline NaYF4:(Yb, Er) infrared-to-visible up-conversion phophors. Nano Lett, 2004, 4: 2191 –2196 Wu G S, Zhang L, Cheng B C, et al. Synthesis of Eu2O3 nanotube arrays through a facile sol-gel template approach. J Am Chem Soc,
2004, 126: 5976–5977 Lu H C, Yi G S, Zhao S Y, et al. Synthesis and characterization of multi-functional nanoparticles possessing magnetic, up-conversion fluorescence and bio-affinity properties. J Mater Chem, 2004, 14: 1336–1341 Sivakumar S, Veggel F, Raudsepp M. Bright white light through up-conversion of a single NIR source from sol-gel-derived thin film made with Ln3+-doped LaF3 nanoparticles. J Am Chem Soc, 2005, 127: 12464–12465 Wu J H, Hao S C, Lin J M, et al. Crystal morphology of anatase titania nanocrystals used in dye-sensitized solar cell. Cryst Growth Des, 2008, 8: 247–252 Lan Z, Wu J H, Lin J M, et al. Influence of molecular weight of PEG on the property of polymer gel electrolyte and performance of quasisolid-state dye-sensitized solar cells. Electrochim Acta, 2007, 52: 6673–6678 Hao S C, Wu J H, Fan L Q, et al. The influence of acid treatment of TiO2 porous film electrode on photoelectric performance of dye-sensitized solar cell. Sol Energy, 2004, 76: 745–750 Wang P, Zakeeruddin S, Comte P, et al. Enhance the performance of dye-sensitized solar cells by co-grafting amphiphilic sensitizer and hexadecylmalonic acid on TiO2 nanocrystals. J Phys Chem B, 2003, 107: 14336–14341 Pang T, Cao W H. Up-conversion luminescence by yttrium tantalate doping Er3+ and co-doping Er3+-Y3+ (in Chinese). Chinese Sci Bull, 2007, 52: 2226–2229 Gratzel M. Perspectives for dye-sensitized nanocrystalline solar cells. Prog Photovoltaic Res Applic, 2000, 8: 171–185 Ito S, Yoshida S, Watanabe T. Fabrication and characterization of meso-macroporous anatase TiO2 films. J Chem Soc Jap, 2000, 73: 1933–1938 Sarmimala H, Peter N, Carmen V, et al. Scattering spherical voids in nanocrystalline TiO2–enhancement of efficiency in dye-sensitized solar cells. Chem Commun, 2005: 2011–2013 Chen S Y, Ting C C, Hsieh W F. Comparison of visible fluorescence properties between sol-gel derived Er3+-Yb3+ and Er3+-Y3+ co-doped TiO2 films. Thin Solid Films, 2003, 434: 171–177 Boyer J, Cuccia L A, Capoianco J A. Synthesis of colloidal upconverting NaYF4:Er3+/Yb3+ and Tm3+/Yb3+ monodisperse nanocrystals. J Am Chem Soc, 2007, 7: 847–852 Li C X, Quan Z W, Yang P P, et al. Shape-controllable synthesis and up-conversion properties of lutetium fluoride (doped with Yb3+/Er3+) microcrystals by hydrothermal process. J Phys Chem C, 2008, 112: 13395–13404 Yu H, Shang Q K, Wang H D, et al. Up-conversion luminescence properties of Er3+ and Yb3+ co-doped TiO2 nanopowders. J Mol Sci, 2007, 23: 118–122 Liu Y, Shen H, Huang X R, et al. A new improved structure of dye-sensitized solar cells with reflection film. Chinese Sci Bull, 2006, 51: 369–373
Open Access This article is distributed under the terms of the Creative Commons Attribution License which permits any use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.